XRD- and infrared-probed anisotropic thermal expansion properties of an organic semiconducting single crystal.
Mohanraj, J.; Capria, E.; Benevoli, L.; Perucchi, A.; Demitri, N.; Fraleoni-Morgera, A; Physical chemistry chemical physics : PCCP 20 (2018) 1984–1992; doi:10.1039/c7cp05209j

data_7229702
_publ_section_title
;
 XRD- and infrared-probed anisotropic thermal expansion properties of an
 organic semiconducting single crystal.
;
_journal_issue                   3
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              1984
_journal_page_last               1992
_journal_paper_doi               10.1039/c7cp05209j
_journal_volume                  20
_journal_year                    2018
_chemical_formula_moiety         'C7 H5 N O'
_chemical_formula_sum            'C7 H5 N O'
_chemical_formula_weight         119.12
_chemical_name_common            4-hydroxycyanobenzene
_space_group_crystal_system      orthorhombic
_space_group_IT_number           60
_space_group_name_Hall           '-P 2n 2ab'
_space_group_name_H-M_alt        'P b c n'
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2013
_audit_update_record
;
2017-06-30 deposited with the CCDC.
2017-12-11 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   9.168(2)
_cell_length_b                   10.677(1)
_cell_length_c                   25.402(1)
_cell_measurement_reflns_used    8947
_cell_measurement_temperature    240(2)
_cell_measurement_theta_max      32.89
_cell_measurement_theta_min      1.86
_cell_volume                     2486.5(6)
_computing_cell_refinement       'XDS (Kabsch, 2010)'
_computing_data_collection       'Elettra XRD1 Data Collection SW'
_computing_data_reduction        'XDS - SCALA (Winn, 2011)'
_computing_molecular_graphics    'Coot (Emsley, 2004)'
_computing_publication_material  enCIFer/publCIF
_computing_structure_refinement  'SHELXL-2012 (Sheldrick, 2015)'
_computing_structure_solution    'Sir2011 (Burla, 2015)'
_diffrn_ambient_temperature      240(2)
_diffrn_measured_fraction_theta_full 0.980
_diffrn_measured_fraction_theta_max 0.966
_diffrn_measurement_device_type
;
'Huber 4-circles Kappa Goniometer, Pilatus 2M detector'
;
_diffrn_measurement_method       'Rotating crystal'
_diffrn_radiation_type           Synchrotron
_diffrn_radiation_wavelength     0.8266
_diffrn_reflns_av_R_equivalents  0.043
_diffrn_reflns_av_unetI/netI     0.0246
_diffrn_reflns_Laue_measured_fraction_full 0.980
_diffrn_reflns_Laue_measured_fraction_max 0.966
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       32
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            13423
_diffrn_reflns_point_group_measured_fraction_full 0.980
_diffrn_reflns_point_group_measured_fraction_max 0.966
_diffrn_reflns_theta_full        29.733
_diffrn_reflns_theta_max         31.102
_diffrn_reflns_theta_min         1.865
_diffrn_source                   'Elettra Synchrotron - XRD1 BL'
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.122
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.273
_exptl_crystal_description       'thick plate'
_exptl_crystal_F_000             992
_exptl_crystal_size_max          1
_exptl_crystal_size_mid          0.5
_exptl_crystal_size_min          0.25
_refine_diff_density_max         0.168
_refine_diff_density_min         -0.177
_refine_diff_density_rms         0.034
_refine_ls_extinction_coef       0.422(14)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.096
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     172
_refine_ls_number_reflns         2463
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.096
_refine_ls_R_factor_all          0.0413
_refine_ls_R_factor_gt           0.0406
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 w=1/[\s^2^(Fo^2^)+(0.0552P)^2^+0.3589P]
 where P=(Fo^2^+2Fc^2^)/3
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1062
_refine_ls_wR_factor_ref         0.1069
_reflns_Friedel_coverage         0.000
_reflns_number_gt                2375
_reflns_number_total             2463
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c7cp05209j2.cif
_cod_data_source_block           4HCB240K
_cod_depositor_comments
'Adding full bibliography for 7229694--7229703.cif.'
_cod_original_cell_volume        2486.5(7)
_cod_database_code               7229702
_shelxl_version_number           2012-9
_shelx_res_checksum              87539